#------------------------------------------------------------------------------
#$Date: 2024-04-25 17:59:02 +0300 (Thu, 25 Apr 2024) $
#$Revision: 291351 $
#$URL: file:///home/coder/svn-repositories/cod/cif/9/00/27/9002766.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9002766
loop_
_publ_author_name
'Liebscher, A.'
'Gottschalk, M.'
'Franz, G.'
_publ_section_title
;
 The substitution Fe-Al and the isosymmetric displacive phase transition
 in synthetic zoisite: A powder X-ray and infrared spectroscopic study
 Sample: Zo3, X(Fe/(Fe+Al-2)) = 0.0
;
_journal_name_full               'American Mineralogist'
_journal_page_first              909
_journal_page_last               921
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al3 Ca2 H O13 Si3'
_chemical_name_mineral           Zoisite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   16.1913
_cell_length_b                   5.5488
_cell_length_c                   10.0320
_cell_formula_units_Z            4
_cell_volume                     901.298
_database_code_amcsd             0002855
_exptl_crystal_density_diffrn    3.348
_cod_original_formula_sum        'Ca2 Al3 Si3 O13 H'
_cod_database_code               9002766
loop_
_space_group_symop_operation_xyz
x,y,z
x,1/2-y,z
-x,1/2+y,-z
1/2-x,1/2+y,1/2+z
1/2+x,1/2-y,1/2-z
1/2+x,y,1/2-z
1/2-x,-y,1/2+z
-x,-y,-z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
CaA1 0.36660 0.25000 0.43760 ?
CaA2 0.45210 0.25000 0.11300 ?
AlM1,2 0.24980 0.99720 0.19050 ?
AlM3 0.10570 0.75000 0.30130 ?
SiT1 0.08170 0.25000 0.10540 ?
SiT2 0.41010 0.75000 0.28160 ?
SiT3 0.16050 0.25000 0.43490 ?
O1 0.13030 -0.00400 0.14340 ?
O2 0.10180 0.01120 0.42880 ?
O3 0.36010 0.99200 0.24390 ?
O4 0.22120 0.75000 0.30160 ?
O5 0.22650 0.25000 0.31150 ?
O6 0.27240 0.75000 0.06000 ?
O7 0.98920 0.25000 0.16360 ?
O8 0.99850 0.75000 0.29650 ?
O9 0.41900 0.75000 0.44250 ?
O10 0.26760 0.25000 0.07410 ?
H 0.26000 0.25000 0.95000 0.05000
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0002855
